Use of Malachite Green Stain as an Auxiliary Technique
For Differentiation of Asbestiform Sepiolite From
International Asbestos Testing Laboratories, Inc. Mount Laurel, NJ
Asbestos, chrysotile, Sepiolite, Malachite Green Stain
Most matrices submitted to environmental laboratories for asbestos analysis are considered
routine and do not present unique analytical challenges. Occasionally, materials are encountered that
contain non-regulated asbestiform minerals which can be misidentified as asbestos. The clay mineral
sepiolite (Mg4Si6O15(OH)2·6H2O) can be asbestiform and is used as a chrysotile ((Mg3Si2O5(OH)4))
substitute in some applications. Asbestiform sepiolite is structurally, compositionally and optically
similar to chrysotile, which can exhibit variability complicating differentiation. The similarity of sepiolite
to chrysotile combined with chrysotile compositional variability can result in false positives. Malachite
Green stain (Faust1) is a relatively simple and quick technique for differentiation of sepiolite from
chrysotile in conjunction with Polarized Light Microscopy (PLM) analysis.
The clay mineral sepiolite was first described in 1847 from an occurrence in Bettolino, Baldissero
Canavese, Torino Province, Piedmont, Italy2. The mineral name is derived from Greek (sepion) due to a
perceived resemblance to porous cuttlefish bone.1 Shortly after its discovery, the ease in which massive
forms could be carved made it suitable for manufacture of meerschaum pipes. Sepiolite is a relatively
uncommon clay mineral, and most deposits are small. Yet, it has been mined since the 1940’s for use in
drilling fluids, kitty litter, polymer fillers, pharmaceutical carriers, joint compounds and pesticides due to
its unique properties3.
In 1989, the United States Environmental Protection Agency (USEPA) issued a ban on asbestos
containing products4. Regulation of chrysotile asbestos in the the late 1980’s meant that manufacturers
needed to find suitable substitutes for numerous applications. Discovery of a few small commercially
viable deposits of asbestiform sepiolite led to testing of physical properties in order to assess feasibility
use of the mineral as a chrysotile substitute5. Research and development over the years has resulted in
the use of fibrous sepiolite for chrysotile in gaskets and other products that once contained chrysotile.
During routine PLM analysis of a gasket, a fibrous mineral was observed at the greater than 1% level.
The mineral was morphologically similar to chrysotile, but had refractive indices slightly lower than is
typical of most chrysotile observed in building materials. A clay stain used to differentiate smectite from
kaolinite was applied to several of the fibrous mineral bundles. Adsorption of the stain indicated that the
mineral was a fibrous clay (sepiolite) asbestos substitute, not chrysotile. In this paper, the similarities that
could result in misidentification of sepiolite as chrysotile and the staining procedure used an auxilary
technique to PLM analysis is discussed.
CHRYSOTILE - SEPIOLITE COMPARISON
Structural and optical data for chrysotile and sepiolite are provided in Table I for comparison.
The first observation to be made from this table is that both minerals are magnesium silicates of similar
chemical composition and structure (columns 2-4). Comparable cell dimensions (column 4) and Mg:Si
ratios (column 5) could result in erroneous identification by energy dispersive x-ray analysis (EDX) and
selected area electron diffraction (SAED) during Transmission Electron Microscopy (TEM) analysis.
TEM differentiaton could be further complicated by acid leaching of chrysotile (reduced Mg:Si ratios,
diffraction degradation) or encounters with chrysotile fibers atypical of of standards.
A comparison of the optical properties of chrysotile and sepiolite (columns 6-10) further
exemplifies how fibrous sepiolite could be misidentified as chrysotile. Sepiolite has birefringence
(column 10), sign of elongation (column 8) and refractive indices (column 6) within the range of accepted
values used for chrysotile identification. Note that chrysotile clearly has compositional variability as
evident from the refractive index ranges of column 6.
Similarity in birefringence and morphology of fibrous sepiolite compared to chrysotile is
provided as Figures 1 through 4. NIST 1866 SRM and Thetford Mines Quebec orthochrysotile are
provided as control examples of morphologic and refractive index variability amongst chrysotile
specimens. Figures 4 and 8 are images of fibrous sepiolite from a gasket for comparison. All specimens
depicted exhibit distinct asbestiform morphology with discrete fibrils, parallel sides, curvature and
splayed ends. The Thetford Mines chrysotile (Figure 2) however, is morphologically more similar to the
sepiolite referenc specimen (Figure 1) than the NBS SRM (Figure 3).
Refractive index comparison by means of Central Stop Dispersion Staining (CSDS) images is
provided as figures 5-9. Differences in the CSDS colors observed for the Thetford Mines Orthochrysotile
(Figure 7) and the NIST 1866 SRM (Figure 8) is an indication of compositional (magnesium content)
variability. An example of change in chrysotile refractive index upon acid leaching as a simulation of
alteration is evident from the lighter blue CSDS color shown in Figure 9. Note that the CSDS color of the
acid leached chrysotile (Figure 9) is similar to that observed for fibrous sepiolite (Figures 5 and 6),
indicating that sepiolite could possibly be miscategorized as altered chrysotile.
Table I: Comparison of Sepiolite-Chrysotile Optical and Structural Properties6
Mineral Formula Lattice Cell Mg:Si Refractive** Optic Sign of 2V Birefringence
System Dimensions Ratio Indices Sign Elongation
Chrysotile Mg3Si2O4(OH)4 Orth a=5.313, 7:10 1.493-1.549 Biaxial Positive 20 0.010
& b=9.12, (alpha) negative -
Mon c=14.64 1.517-1.571 60
Sepiolite Mg4Si4O15.6H2O Orth a=13.43, 5:10 1.52 (alpha) Biaxial Positive 20 0.010
b=26.88 1.53 (gamma) negative -
* Data from webmineral.com, mindata.org, NVLAP and Handbook of Mineralogy
**Refractive index data for chrysotile included NVLAP range for acid treated/affected specimens
MALACHITE GREEN STAIN TECHNIQUE
Visual differentiation of minerals in thin section by optical microscopy using staining techniques
was routine laboratory procedure in the 1940’s and 1950’s7,8,9. Mineral stain research proliferated with
particular emphasis on clays due to inherently small particle size that make speciation by optical
properties alone difficult. It was during this time period that Faust 1 developed a simple technique for
differentiating kaolinite (non-swelling clay) from montmorillonite (a smectite, swelling clay) using a
dilute solution of malachite green in nitrobenzene after acidification. In the procedure, clay is dispersed
in 10% HCl, an aliquot of the slurry is placed on a microscope slide and taken to dryness on a hot plate at
approximately 1100C. A drop of malachite green in nitrobenzene is placed on the acidified clay,
dispersed, and washed to remove excess dye. Faust found that clays with exchangeable cations such as
montmorillonite adsorb malachite green and turn green is color. Clays such as kaolinite with little or no
exchangeable cations and less adsorption capacity turn yellow. Use of the stain appears to have received
little notice until the 1970’s, when Palenik10 extended its application for particle identification using
microchemical techniques in forensic investigations.
DIFFERENTIATING SEPIOLITE FROM CHRYSOTILE WITH MALACHITE GREEN STAIN
Although sepiolite is a non-swelling clay, it possesses high surface area and porosity due to a
tubular zeolitic water channel in its fibrous structure. The structure of sepiolite accounts for greater
adsorptive and absorptive capacity than non-swelling clays such as kaolinite. Application of the
malachite green stain on sepiolite from a gasket and the Quincy Sur Cher sepiolite control produced a
deep bluish green color (Figure 10 and 11). Unaltered chrysotile (no acid leaching) is not sorbtive and
does not stain (Figure 12). Chrysotile exposed to concentrated HCl for prolonged periods (24hrs +)
results in higher stain sorptive capacity due to leaching of magnesium after application of the stain
(Figure 13). The color of the stain, however, is of a slightly grayish hue and is uneven, suggestive of
alteration effects, not structural staining.
Sepiolite is a fibrous clay mineral that can crystallize in an asbestiform habit. The physical
properties of asbestiform sepiolite make it useful as an asbestos substitute for some applications. The
structural, chemical and optical properties are similar to chrysotile, which can lead to false positives by
analysts not familiar with sepiolite. Utilization of malachite green stain following the Faust technique can
serve as a useful and quick auxiliary technique to PLM analysis for differentiating sepiolite from
chrysotile in some instances. Chrysotile affected by acid leaching may present an interference as it can
sorb malachite green stain. Comparison of reference slides used as controls, however, should facilitate
differentiation sepiolite from acid leached/altered chrysotile during staining investigations.
1. Faust, G.T. Staining of clay minerals as a rapid means of identification in natural and beneficiated products. U.S.
Bureau of Mines, Report of Investigation of Mines, 3522, 1940.
2.Glocker, E.F. (1847): Generum et specierum mineralium secundum ordines naturales digestorium synopsis. Halle,
3. 40 CFR Part 763-Asbestos.
4-Handbook of Clay Science. F. Bergaya, B.K.G. Theng and G. Lagaly, Eds. 1 Edition, Elsevier, 2006.
5-Russell, A. (1991) Specialty clays: market niches taken by unique properties. lnd. Miner., June,
6-Handbook of Mineralogy.Anthony, Bideaux, Bladh,Nichols. Volume III, Minerlaogical Society of
7-A Quantitative Color Test for Rapid Identification of Clay Mineral Groups. Hambledon and Dodd,
1953. Econ. Geology, V.48, #2, 139-146.
8-The Identification of Montmorillonoids in Clay. R. Greene and Kelly, 1953. Eur. Jour. Of Soil Science.
Vol 4, #2, 232-237.
9-Friedman, G.M. 1959 Identification of carbonate minerals by staining techniques. J. Sed. Petrology 29:87-97
10-Palenik S.J, 1979. Microchemical Reactions In Particle Identification. The Particle Atlas, Edition Two, Volume 5.
Figure 1. Image of Quincy-Sur-Cher, Fr. Fibrous sepiolite reference. Crossed Polarized Light,
Figure 4. Image of sepiolite bundle removed from gasket. 100X,
Crossed polarized light.
Figure 5. Image of Quincy Sur Sepiolite, CSDS, 100X, 1.550 Cargille Series E.
Figure 6. Image of sepiolite from gasket. CSDS, 100X, 1.550 Cargille Series E.
Figure 7. Image of Thetford Mines, Quebec Canada orthochrysotile, CSDS, 100X, 1.550 Cargille Series E.
Figure 8. Image of NIST SRM 1866 Chrysotile, CSDS, 100X, 1.550 Cargille Series E.
Figure 9. Image of NIST SRM 1866 Chrysotile after 24 hours in concentrated HCl, CSDS, 100X, 1.550
Cargille Series E.
Figure 10. Malachite green stained sepiolite from gasket. 100X,
Plane polarized light.
Figure 11. Malachite green stained Quincy Sur Cher sepiolite control, 100x, plane polarized light.
Figure 12. Thetford mines chrysotile showing lack of stain sorbtion.
100x, plane polarized light.
Figure 13. Malachite green stained NIST SRM 1866 chrysotile leached for 24 hrs.
Plane polarized light, 100X.